Download presentation

Presentation is loading. Please wait.

1
**Grain Boundary Properties: Energy (L21)**

27-750, Fall 2009 Texture, Microstructure & Anisotropy A.D. Rollett, P.N. Kalu With thanks to: G.S. Rohrer, D. Saylor, C.S. Kim, K. Barmak, others … Updated 19th Nov. ‘09

2
References Interfaces in Crystalline Materials, Sutton & Balluffi, Oxford U.P., Very complete compendium on interfaces. Interfaces in Materials, J. Howe, Wiley, Useful general text at the upper undergraduate/graduate level. Grain Boundary Migration in Metals, G. Gottstein and L. Shvindlerman, CRC Press, The most complete review on grain boundary migration and mobility. Materials Interfaces: Atomic-Level Structure & Properties, D. Wolf & S. Yip, Chapman & Hall, 1992. See also mimp.materials.cmu.edu (Publications) for recent papers on grain boundary energy by researchers connected with the Mesoscale Interface Mapping Project (“MIMP”).

3
**Outline Motivation, examples of anisotropic grain boundary properties**

Grain boundary energy Measurement methods Surface Grooves Low angle boundaries High angle boundaries Boundary plane vs. CSL Herring relations, Young’s Law Extraction of GB energy from dihedral angles Capillarity Vector Simulation of grain growth

4
**Why learn about grain boundary properties?**

Many aspects of materials processing, properties and performance are affected by grain boundary properties. Examples include: - stress corrosion cracking in Pb battery electrodes, Ni-alloy nuclear fuel containment, steam generator tubes, aerospace aluminum alloys - creep strength in high service temperature alloys - weld cracking (under investigation) - electromigration resistance (interconnects) Grain growth and recrystallization Precipitation of second phases at grain boundaries depends on interface energy (& structure).

5
**Properties, phenomena of interest**

1. Energy (excess free energy grain growth, coarsening, wetting, precipitation) 2. Mobility (normal motion grain growth, recrystallization) 3. Sliding (tangential motion creep) 4. Cracking resistance (intergranular fracture) 5. Segregation of impurities (embrittlement, formation of second phases)

6
**Grain Boundary Diffusion**

Especially for high symmetry boundaries, there is a very strong anisotropy of diffusion coefficients as a function of boundary type. This example is for Zn diffusing in a series of <110> symmetric tilts in copper. Note the low diffusion rates along low energy boundaries, especially 3.

7
**Grain Boundary Sliding**

640°C Grain boundary sliding should be very structure dependent. Reasonable therefore that Biscondi’s results show that the rate at which boundaries slide is highly dependent on misorientation; in fact there is a threshold effect with no sliding below a certain misorientation at a given temperature. 600°C 500°C Biscondi, M. and C. Goux (1968). "Fluage intergranulaire de bicristaux orientés d'aluminium." Mémoires Scientifiques Revue de Métallurgie 55(2):

8
**Grain Boundary Energy: Definition**

Grain boundary energy is defined as the excess free energy associated with the presence of a grain boundary, with the perfect lattice as the reference point. A thought experiment provides a means of quantifying GB energy, g. Take a patch of boundary with area A, and increase its area by dA. The grain boundary energy is the proportionality constant between the increment in total system energy and the increment in area. This we write: g = dG/dA The physical reason for the existence of a (positive) GB energy is misfit between atoms across the boundary. The deviation of atom positions from the perfect lattice leads to a higher energy state. Wolf established that GB energy is correlated with excess volume in an interface. There is no simple method, however, for predicting the excess volume.

9
**Measurement of GB Energy**

We need to be able to measure grain boundary energy. In general, we do not need to know the absolute value of the energy but only how it varies with boundary type, i.e. with the crystallographic nature of the boundary. For measurement of the anisotropy of the energy, then, we rely on local equilibrium at junctions between boundaries. This can be thought of as a force balance at the junctions. For not too extreme anisotropies, the junctions always occur as triple lines.

10
**Experimental Methods for g.b. energy measurement**

G. Gottstein & L. Shvindlerman, Grain Boundary Migration in Metals, CRC (1999) Method (a), with dihedral angles at triple lines, is most generally useful; method (c), with surface grooving also used.

11
Zero-creep Method The zero-creep experiment primarily measures the surface energy. The surface energy tends to make a wire shrink so as to minimize its surface energy. An external force (the weight) tends to elongate the wire. Varying the weight can vary the extension rate from positive to negative, permitting the zero-creep point to be interpolated. Grain boundaries perpendicular to the wire axis counteract the surface tension effect by tending to decrease the wire diameter.

12
Herring Equations We can demonstrate the effect of interfacial energies at the (triple) junctions of boundaries. Equal g.b. energies on 3 GBs implies equal dihedral angles: 1 g1=g2=g3 2 3 120°

13
**Definition of Dihedral Angle**

Dihedral angle, c:= angle between the tangents to an adjacent pair of boundaries (unsigned). In a triple junction, the dihedral angle is assigned to the opposing boundary. 1 g1=g2=g3 2 3 120° c1 : dihedral angle for g.b.1

14
Dihedral Angles An material with uniform grain boundary energy should have dihedral angles equal to 120°. Likely in real materials? No! Low angle boundaries (crystalline materials) always have a dislocation structure and therefore a monotonic increase in energy with misorientation angle (Read-Shockley model). The inset figure is taken from a paper in preparation by Prof. K. Barmak and shows the distribution of dihedral angles measured in a 0.1 µm thick film of Al, along with a calculated distribution based on an GB energy function from a similar film (with two different assumptions about the distribution of misorientations).

15
**Unequal energies c1>120° 1 g1<g2=g3 2 3**

If the interfacial energies are not equal, then the dihedral angles change. A low g.b. energy on boundary 1 increases the corresponding dihedral angle. 1 g1<g2=g3 2 3 c1>120°

16
**Unequal Energies, contd.**

A high g.b. energy on boundary 1 decreases the corresponding dihedral angle. Note that the dihedral angles depend on all the energies. 1 g1>g2=g3 3 2 c1< 120°

17
Wetting For a large enough ratio, wetting can occur, i.e. replacement of one boundary by the other two at the TJ. g1>g2=g3 Balance vertical forces g1 = 2g2cos(c1/2) Wetting g1 2 g2 g1 1 g2cosc1/2 g3cosc1/2 3 2 c1< 120°

18
**Triple Junction Quantities**

Diagram of a labeling convention for grain boundary character, showing dihedral angles, c, inclination angles, f, boundary tangent vectors, b, boundary normals, n, and grain orientations, g. The triple junction line is perpendicular to the plane of the diagram.

19
**Triple Junction Quantities**

Grain boundary tangent (at a TJ): b Grain boundary normal (at a TJ): n Grain boundary inclination, measured anti-clockwise with respect to a(n arbitrarily chosen) reference direction (at a TJ): f Grain boundary dihedral angle: c Grain orientation:g

20
**Force Balance Equations/ Herring Equations**

The Herring equations[(1951). Surface tension as a motivation for sintering. The Physics of Powder Metallurgy. New York, McGraw-Hill Book Co.: ] are force balance equations at a TJ. They rely on a local equilibrium in terms of free energy. A virtual displacement, dr, of the TJ (L in the figure) results in no change in free energy. See also: Kinderlehrer D and Liu C, Mathematical Models and Methods in Applied Sciences, (2001) ; Kinderlehrer, D., Lee, J., Livshits, I., and Ta'asan, S. (2004) Mesoscale simulation of grain growth, in Continuum Scale Simulation of Engineering Materials, (Raabe, D. et al., eds),Wiley-VCH Verlag, Weinheim, Chap. 16,

21
**Derivation of Herring Equs.**

A virtual displacement, dr, of the TJ results in no change in free energy. See also: Kinderlehrer, D and Liu, C Mathematical Models and Methods in Applied Sciences {2001} ; Kinderlehrer, D., Lee, J., Livshits, I., and Ta'asan, S. 2004 Mesoscale simulation of grain growth, in Continuum Scale Simulation of Engineering Materials, (Raabe, D. et al., eds), Wiley-VCH Verlag, Weinheim, Chapt. 16,

22
Force Balance Consider only interfacial energy: vector sum of the forces must be zero to satisfy equilibrium. These equations can be rearranged to give the Young equations (sine law):

23
**Analysis of Thermal Grooves**

Surface Crystal 2 W Ψs Crystal 1 d ? β 2W Surface 1 Surface 2 Grain Boundary γGb γS2 γS1 It is often reasonable to assume a constant surface energy, gS, and examine the variation in GB energy, gGb, as it affects the thermal groove angles

24
**Grain Boundary Energy Distribution is Affected by Composition**

Δγ = 1.09 1 m Δγ = 0.46 This anisotropy was confirmed by thermal groove measurements, which showed that the doped sample had a wider distribution of thermal groove widths and, therefore a wider distribution of energies. The diagram in lower right shows how we apply Young’s Eq, i.e. same local eq. at TJs to the balance between surfaces and GB energy. Image in upper right is an AFM of thermally grooved GBs. Ca solute increases the range of the gGB/gS ratio. The variation of the relative energy in undoped MgO is lower (narrower distribution) than in the case of doped material. 76

25
**Bi impurities in Ni have the opposite effect**

Pure Ni, grain size: 20mm The opposite trend was found in Bi-doped Ni. In this case, Bi suppressed the grain boundary anisotropy and a narrower range of energies was found. Very curious: Cu-Bi exhibits the opposite effect – the doped case is WIDER than the undoped. So, it is NOT possible to assume that segregation decreases or increases the anisotropy of GB energy. Bi-doped Ni, grain size: 21mm Range of gGB/gS (on log scale) is smaller for Bi-doped Ni than for pure Ni, indicating smaller anisotropy of gGB/gS. This correlates with the plane distribution 77

26
**G.B. Properties Overview: Energy**

Low angle boundaries can be treated as dislocation structures, as analyzed by Read & Shockley (1951). Grain boundary energy can be constructed as the average of the two surface energies - gGB = g(hklA)+g(hklB). For example, in fcc metals, low energy boundaries are found with {111} terminating surfaces. Does mobility scale with g.b. energy, based on a dependence on acceptor/donor sites? Read-Shockley one {111} two {111} planes (3 …) Shockley W, Read WT. Quantitative Predictions From Dislocation Models Of Crystal Grain Boundaries. Phys. Rev. 1949;75:692.

27
**Grain boundary energy: current status?**

Limited information available: Deep cusps exist for a few <110> CSL types in fcc (S3, S11), based on both experiments and simulation. Extensive simulation results [Wolf et al.] indicate that interfacial free volume is good predictor. No simple rules available, however, to predict free volume. Wetting results in iron [Takashima, Wynblatt] suggest that a broken bond approach (with free volume and twist angle) provides a reasonable 5-parameter model. If binding energy is neglected, an average of the surface energies is a good predictor of grain boundary energy in MgO [Saylor, Rohrer]. Minimum dislocation density structures [Frank - see description in Sutton & Balluffi] provide a good model of g.b. energy in MgO, and may provide a good model of low angle grain boundary mobility.

28
Grain Boundary Energy First categorization of boundary type is into low-angle versus high-angle boundaries. Typical value in cubic materials is 15° for the misorientation angle. Typical values of g.b. energies vary from J.m-2 for Al to 0.87 for Ni J.m-2 (related to bond strength, which is related to melting point). Read-Shockley model describes the energy variation with angle for low-angle boundaries successfully in many experimental cases, based on a dislocation structure.

29
Read-Shockley model Start with a symmetric tilt boundary composed of a wall of infinitely straight, parallel edge dislocations (e.g. based on a 100, 111 or 110 rotation axis with the planes symmetrically disposed). Dislocation density (L-1) given by: 1/D = 2sin(q/2)/b q/b for small angles.

30
Tilt boundary b D Each dislocation accommodates the mismatch between the two lattices; for a <112> or <111> misorientation axis in the boundary plane, only one type of dislocation (a single Burgers vector) is required.

31
Read-Shockley contd. For an infinite array of edge dislocations the long-range stress field depends on the spacing. Therefore given the dislocation density and the core energy of the dislocations, the energy of the wall (boundary) is estimated (r0 sets the core energy of the dislocation): ggb = E0 q(A0 - lnq), where E0 = µb/4π(1-n); A0 = 1 + ln(b/2πr0)

32
**LAGB experimental results**

Experimental results on copper. Note the lack of evidence of deep minima (cusps) in energy at CSL boundary types in the <001> tilt or twist boundaries. Disordered Structure Dislocation Structure [Gjostein & Rhines, Acta metall. 7, 319 (1959)]

33
Read-Shockley contd. If the non-linear form for the dislocation spacing is used, we obtain a sine-law variation (Ucore= core energy): ggb = sin|q| {Ucore/b - µb2/4π(1-n) ln(sin|q|)} Note: this form of energy variation may also be applied to CSL-vicinal boundaries.

34
**Energy of High Angle Boundaries**

No universal theory exists to describe the energy of HAGBs. Based on a disordered atomic structure for general high angle boundaries, we expect that the g.b. energy should be at a maximum and approximately constant. Abundant experimental evidence for special boundaries at (a small number) of certain orientations for which the atomic fit is better than in general high angle g.b’s. Each special point (in misorientation space) expected to have a cusp in energy, similar to zero-boundary case but with non-zero energy at the bottom of the cusp. Atomistic simulations suggest that g.b. energy is (positively) correlated with free volume at the interface.

35
**Exptl. vs. Computed Egb <100> Tilts <110> Tilts**

Note the presence of local minima in the <110> series, but not in the <100> series of tilt boundaries. S11 with (311) plane <110> Tilts S3, 111 plane: CoherentTwin Hasson & Goux, Scripta metall

36
**Surface Energies vs. Grain Boundary Energy**

A recently revived, but still controversial idea, is that the grain boundary energy is largely determined by the energy of the two surfaces that make up the boundary (and that the twist angle is not significant). This is has been demonstrated to be highly accurate in the case of MgO, which is an ionic ceramic with a rock-salt structure. In this case, {100} has the lowest surface energy, so boundaries with a {100} plane are expected to be low energy. The next slide, taken from the PhD thesis work of David Saylor, shows a comparison of the g.b. energy computed as the average of the two surface energies, compared to the frequency of boundaries of the corresponding type. As predicted, the frequency is lowest for the highest energy boundaries, and vice versa.

37
**l(n) 2-parameter distributions: boundary normal only**

j l(n) (MRD) • Index n’ in the crystal reference frame: n = gin' and n = gi+1n' (2 parameter description) rij2 j 1 2 3 rij1 n’ij l’ij

38
**Physical Meaning of Grain Boundary Parameters**

q gB gA Lattice Misorientation, ∆g (rotation, 3 parameters) Boundary Plane Normal, n (unit vector, 2 parameters) Grain Boundaries have 5 Macroscopic Degrees of Freedom

39
**Tilt versus Twist Boundaries**

Isolated/occluded grain (one grain enclosed within another) illustrates variation in boundary plane for constant misorientation. The normal is // misorientation axis for a twist boundary whereas for a tilt boundary, the normal is to the misorientation axis. Many variations are possible for any given boundary. Misorientation axis Twist boundaries Tilt boundaries gA gB

40
Separation of ∆g and n Plotting the boundary plane requires a full hemisphere which projects as a circle. Each projection describes the variation at fixed misorientation. Any (numerically) convenient discretization of misorientation and boundary plane space can be used. Distribution of normals for boundaries with S3 misorientation (commercial purity Al) Misorientation axis, e.g. 111, also the twist type location

41
**Grain Boundary Distribution in MgO: [100] l(Dg, n)**

^ [100] l(n|5°/[100]) n ^ n ^ l(n|15°/[100]) n ^ l(n|25°/[100]) For any point on the plots, we have to define the BP normal in terms of its crystallographic direction The problem is that, we can express it in terms of either of the two crystals, for example … blue = 100, red does not, we have to pick one We see that there are always peaks in the distribution for <100> BP normals, as it turns out that the other peaks occur when the BP normal is <100> in terms of the other crystal that we are not plotting So, we start with one peak at each of the <100> poles when the <100> planes are reasonably close to each other, as the misorientation angle increases these planes move away from each other, and when the <100> planes of the two crystals are far enough from each other the peak splits Not counting the low angle boundaries, every peak in the movie corresponds to a GB that has one of the two possible crystallographic BP normal directions is near <100> n ^ l(n|35°/[100]) Every peak in l(Dg,n) is related to a boundary with a {100} plane

42
**Grain Boundary Population (Dg averaged)**

Examples of 2-Parameter Distributions Grain Boundary Population (Dg averaged) Measured Surface Energies Saylor & Rohrer, Inter. Sci. 9 (2001) 35. MgO SrTiO3 Sano et al., J. Amer. Ceram. Soc., 86 (2003) 1933.

43
**Grain boundary energy and population**

For all grain boundaries in MgO 0.0 0.5 1.0 1.5 2.0 2.5 3.0 0.70 0.78 0.86 0.94 1.02 ggb (a.u) ln(l+1) Population and Energy are inversely correlated Saylor DM, Morawiec A, Rohrer GS. Distribution and Energies of Grain Boundaries as a Function of Five Degrees of Freedom. Journal of The American Ceramic Society 2002;85: Capillarity vector used to calculate the grain boundary energy distribution – see later slides.

44
**Grain boundary energy and population**

[100] misorientations in MgO Grain boundary energy g(n|w/[100]) w= 10° w= 30° w=10° MRD w= 30° Grain boundary distribution l(n|w/[100]) Population and Energy are inversely correlated Saylor, Morawiec, Rohrer, Acta Mater. 51 (2003) 3675

45
**Boundary energy and population in Al**

0.2 0.4 0.6 0.8 30 60 90 120 150 180 Energy, a.u. Misorientation angle, deg. 10 5 15 25 20 l(Dg, n), MRD S= 9 11 3 Symmetric [110] tilt boundaries Energies: G.C. Hasson and C. Goux Scripta Met. 5 (1971) 889. Al boundary populations: Saylor et al. Acta mater., 52, (2004).

46
**S5 (37°/[100]) tilt boundaries in MgO**

ggb (a.u) q010 (°) l (MRD) (012) (021) (043) (010) 0.87 0.88 0.89 0.90 0.91 30 60 90 120 150 180 0.30 0.35 0.40 0.45 0.50 0.55 (031) (001) (034) (013) g The energy-population correlation is not one-to-one

47
**Inclination Dependence**

Interfacial energy can depend on inclination, i.e. which crystallographic plane is involved. Example? The coherent twin boundary is obviously low energy as compared to the incoherent twin boundary (e.g. Cu, Ag). The misorientation (60° about <111>) is the same, so inclination is the only difference.

48
**Twin: coherent vs. incoherent**

Porter & Easterling fig. 3.12/p123

49
The torque term Change in inclination causes a change in its energy, tending to twist it (either back or forwards) df 1

50
**Inclination Dependence, contd.**

For local equilibrium at a TJ, what matters is the rate of change of energy with inclination, i.e. the torque on the boundary. Recall that the virtual displacement twists each boundary, i.e. changes its inclination. Re-express the force balance as (sg): torque terms surface tension terms

51
Herring’s Relations

52
Torque effects The effect of inclination seems esoteric: should one be concerned about it? Yes! Twin boundaries are only one example where inclination has an obvious effect. Other types of grain boundary (to be explored later) also have low energies at unique misorientations. Torque effects can result in inequalities* instead of equalities for dihedral angles, if one of the boundaries is in a cusp, such as for the coherent twin. * B.L. Adams, et al. (1999). “Extracting Grain Boundary and Surface Energy from Measurement of Triple Junction Geometry.” Interface Science 7:

53
**Aluminum foil, cross section**

surface Torque term literally twists the boundary away from being perpendicular to the surface Cross-section of a thin foil of Al.

54
**Why Triple Junctions? 90° 120°**

For isotropic g.b. energy, 4-fold junctions split into two 3-fold junctions with a reduction in free energy: 90° 120°

55
**How to Measure Dihedral Angles and Curvatures: 2D microstructures**

Image Processing (1) (2) Fit conic sections to each grain boundary: Q(x,y)=Ax2+ Bxy+ Cy2+ Dx+ Ey+F = 0 Assume a quadratic curve is adequate to describe the shape of a grain boundary. [PhD thesis, CMU, CC Yang 2001]

56
**Measuring Dihedral Angles and Curvatures**

(3) Calculate the tangent angle and curvature at a triple junction from the fitted conic function, Q(x,y): Q(x,y)=Ax2+ Bxy + Cy2+ Dx+ Ey+F=0

57
**Calculation of G.B. Energy**

In principle, one can measure many different triple junctions to characterize crystallography, dihedral angles and curvature. From these measurements one can extract the relative properties of the grain boundaries. The simpler procedure, described here, uses the dihedral angles and calculates the GB energy based on the 3 parameters of misorientation only, i.e. neglecting the torque term. The more complete calculation of GB energy is performed for all 5 macroscopic degrees of freedom. Since this does include the torque term, the capillarity vector can be used to accomplish this. The concept of the capillarity vector is described in subsequent slides.

58
Energy Extraction (sin2) 1 - (sin1) 2 = 0 (sin3) 2 - (sin2) 3 = 0 sin2 -sin …0 sin3 -sin * * * * 0 1 2 3 n = 0 Measurements at many TJs; bin the dihedral angles by g.b. type; average the sinci; each TJ gives a pair of equations • PhD thesis, CMU, CC Yang 2001. • D. Kinderlehrer, et al. , Proc. of the Twelfth International Conference on Textures of Materials, Montréal, Canada, (1999) 1643. • K. Barmak, et al., "Grain boundary energy and grain growth in Al films: Comparison of experiments and simulations", Scripta materialia, 54 (2006) : following slides …

59
**Example: {001}c [001]s textured Al foil**

Determination of Grain Boundary Energy via a Statistical Multiscale Analysis Method Assume: Equilibrium at the triple junction (TJ) Grain boundary energy to be independent of grain boundary inclination Sort boundaries according to misorientation angle () – use 2o bins Symmetry constraint: 62.8o Type Misorientation Angle 1 1.1-4 2 4.1-6 3 6.1-8 4 8.1-10 5 6 7 8 9 10 11 12 13 q - misorientation angle c - dihedral angle K. Barmak, et al. Example: {001}c [001]s textured Al foil

60
**Equilibrium at Triple Junctions**

Herring’s Eq. Young’s Eq. bj - boundary tangent nj - boundary normal c - dihedral angle s - grain boundary energy Example: {001}c [001]s textured Al foil Since the crystals have strong {111} fiber texture, we assume ; - all grain boundaries are pure {111} tilt boundaries - the tilt angle is the same as the misorientation angle To measure lines, triple junctions and dihedral angles, one can use Linefollow (S. Mahadevan and D. Casasent: Proc. SPIE, 2001, pp ) K. Barmak, et al.

61
**Cross-Sections Using OIM**

3 mm [001] inverse pole figure map, raw data SEM image [001] inverse pole figure map, cropped cleaned data - remove Cu (~0.1 mm) - clean up using a grain dilation method (min. pixel 10) Al film [010] sample [001] sample scanned cross-section [010] inverse pole figure map, cropped cleaned data Nearly columnar grain structure more examples 3 mm K. Barmak, et al.

62
**Grain Boundary Energy Calculation : Method**

Type 1 Type 1 - Type 2 = Type 2 - Type 1 Type 2 - Type 3 = Type 3 - Type 2 Type 1 - Type 3 = Type 3 - Type 1 c2 Type 3 Type 2 Pair boundaries and put into urns of pairs Linear, homogeneous equations Young’s Equation K. Barmak, et al.

63
**Grain Boundary Energy Calculation : Method**

N×(N-1)/2 equations N unknowns i=1,….,N(N-1)/2 N(N-1)/2 N = K. Barmak, et al.

64
**Grain Boundary Energy Calculation : Summary**

Assuming columnar grain structure and pure <111> tilt boundaries # of total TJs : 8694 # of {111} TJs : 7367 (10 resolution) 22101 (=7367×3) boundaries calculation of dihedral angles - reconstructed boundary line segments from TSL software 2 binning (0-1, 1 -3, 3 -5, …,59 -61,61 -62) 32×31/2=496 pairs no data at low angle boundaries (<7) i=1,….,N(N-1)/2 Kaczmarz iteration method B.L. Adams, D. Kinderlehrer, W.W. Mullins, A.D. Rollett, and Shlomo Ta’asan, Scripta Mater. 38, 531 (1998) Reconstructed boundaries K. Barmak, et al.

65
**<111> Tilt Boundaries: Results**

2 3 4 5 6 . 8 Relative Boundary Energy M i s o r e n t a A g S7 S13 l e , o Cusps at tilt angles of 28 and 38 degrees, corresponding to CSL type boundaries S13 and S7, respectively. Remember that boundaries in a strongly <111> textured thin film are constrained to be 111 tilt boundaries. K. Barmak, et al.

66
Capillarity Vector The capillarity vector is a convenient quantity to use in force balances at junctions of surfaces. It is derived from the variation in (excess free) energy of a surface. In effect, the capillarity vector combines both the surface tension (so-called) and the torque terms into a single vector quantity. The vector sum of the capillarity vectors of three boundaries joined at a triple line must (vector) sum to zero, or, more precisely, the vector sum cross the line tangent must be zero. It is therefore feasible to construct an algorithm that computes the anisotropy of grain boundary energy based on (iteratively) minimizing the error of the above vector sum at all triple lines.

67
Equilibrium at TJ The utility of the capillarity vector, x, can be illustrated by re-writing Herring’s equations as follows, where l123 is the triple line (tangent) vector. (x1 + x2 + x3) x l123 = 0 Note that the cross product with the triple line tangent implies resolution of forces perpendicular to the triple line. Used by the MIMP group to calculate the GB energy function for MgO, based on a dataset with boundary normals (which imply dihedral angles) and grain orientations: Morawiec A. Method to calculate the grain boundary energy distribution over the space of macroscopic boundary parameters from the geometry of triple junctions. Acta mater. 2000;48:3525. Also, Saylor DM, Morawiec A, Rohrer GS. Distribution and Energies of Grain Boundaries as a Function of Five Degrees of Freedom. Journal of The American Ceramic Society 2002;85:3081.

68
**Capillarity vector definition**

Following Hoffman & Cahn, define a unit surface normal vector to the surface, , and a scalar field, rg( ), where r is a radius from the origin. Typically, the normal is defined w.r.t. crystal axes. “A vector thermodynamics for anisotropic surfaces. I. Fundamentals and application to plane surface junctions.”, D.W. Hoffman and J.W. Cahn, Surface Science 31: (1972). Also read sections & in Sutton & Balluffi.

69
**Capillarity vector: derivations**

Definition: From which, Eq (1) Giving, Compare with the rule for products: gives: (2), and, (3) Combining total derivative of (2), with (3): Eq (4):

70
**Capillarity vector: components**

The physical consequence of Eq (2) is that the component of x that is normal to the associated surface, xn, is equal to the surface energy, g. Can also define a tangential component of the vector, xt, that is parallel to the surface: where the tangent vector is associated with the maximum rate of change of energy. Sutton & Balluffi show how to derive the capillary pressure associated with a boundary from the capillarity vector. The result is the same as Herring’s original derivation and involves the “mean curvature”, k1+k2, (which is not the average curvature!), the mobility and the “interface stiffness”, which is the sum of the GB energy and its second derivative with respect to inclination. In this approach, principal curvatures must be evaluated, which is inconvenient for numerical calculations.

71
**Computer Simulation of Grain Growth**

Simulation of Grain Growth and G.B. populations Computer Simulation of Grain Growth From the PhD thesis project of Jason Gruber. MgO-like grain boundary properties were incorporated into a finite element model of grain growth, i.e. minima in energy for any boundary with a {100} plane on either side. Simulated grain growth leads to the development of a g.b. population that mimics the experimental observations very closely. The result demonstrates that it is reasonable to expect that an anisotropic GB energy will lead to a stable population of GB types (GBCD).

72
**Moving Finite Element Method**

Grain Growth Simulations with Grain 3D A.P. Kuprat: SIAM J. Sci. Comput. 22 (2000) Gradient Weighted Moving Finite Elements (LANL); PhD by Jason Gruber Elements move with a velocity that is proportional to the mean curvature Initial mesh: 2,578 grains, random grain orientations (16 x 2,578 = 41,248) Energy anisotropy modeled after that observed for magnesia: minima on {100}.

73
**GWMFE Results Grain 3D Simulations l(n) t=0 t=3 t=5 t=15 t=10 t=1**

MRD t=0 • Input energy modeled after MgO • Steady state population develops that correlates (inversely) with energy. t=1 t=5 t=10 t=15 t=3 0.8 1 1.2 1.4 1.6 1 10 4 2 10 3 10 4 10 5 10 5 10 15 20 25 l (MRD) l(111) l(100) l(100)/l(111) Grains number of grains time step

74
**Population versus Energy**

Correlation of Grain Boundary Energy and Population Simulated data: Moving finite elements -3 -2 -1 1 2 3 0.7 0.75 0.8 0.85 0.9 0.95 1.05 ln(l) ggb (a.u.) (a) Experimental data: MgO -3 -2 -1 1 1.05 1.1 1.15 1.2 1.25 ln(l) ggb (a.u.) (b) The relationship between the energy and the distribution the results from the simulation is also similar to the experiment. One of the most important issues we intend to investigate is how this scales with properties and how universal it is. Energy and population are strongly correlated in both experimental results and simulated results. Is there a universal relationship?

75
G.B. Energy: Summary For low angle boundaries, use the Read-Shockley model with a logarithmic dependence: well established both experimentally and theoretically. For high angle boundaries, use a constant value unless near a CSL structure with high fraction of coincident sites and plane suitable for good atomic fit. In ionic solids, a good approximation for the grain boundary energy is simply the average of the two surface energies (modified for low angle boundaries). This approach appears to be valid for metals also. In fcc metals, for example, low energy boundaries are associated with the presence of the close-packed 111 surface on one or both sides of the boundary. There are a few CSL types with special properties, e.g. high mobility sigma-7 boundaries in fcc metals.

76
Summary, contd. Although the CSL theory is a useful introduction to what makes certain boundaries have special properties, grain boundary energy appears to be more closely related to the energies of the two surfaces comprising the boundary. This holds over a wide range of substances. Grain boundary populations are inversely related to the associated energies. Grain boundary energies can be calculated from data on triple junctions that includes boundary normals and grain orientations.

77
Supplemental Slides

78
**Young Equns, with Torques**

Contrast the capillarity vector expression with the expanded Young eqns.:

79
**Expanded Young Equations**

Project the force balance along each grain boundary normal in turn, so as to eliminate one tangent term at a time:

Similar presentations

OK

Dependence of Grain Boundary Mobility on Boundary Plane Hao Zhang 1, Mikhail Mendelev 1,2 and David Srolovitz 1 1 PRISM, Princeton University 2 Ames Laboratory.

Dependence of Grain Boundary Mobility on Boundary Plane Hao Zhang 1, Mikhail Mendelev 1,2 and David Srolovitz 1 1 PRISM, Princeton University 2 Ames Laboratory.

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on case study of cyber crime Ppt on genders for grade 1 Ppt on hvdc circuit breaker Ppt on high voltage engineering corporation Ppt on natural resources and conservation degree Ppt on building information modeling training Ppt on cross cultural communication barriers Ppt on single phase transformer Ppt on earth and space book Ppt on nitrogen cycle and nitrogen fixation examples